- Email: [email protected]

Contents lists available at ScienceDirect

CIRP Annals - Manufacturing Technology jou rnal homep age : ht t p: // ees .e lse vi er . com /ci r p/ def a ult . asp

Optimization of the stream ﬁnishing process for mechanical surface treatment by numerical and experimental process analysis Frederik Zanger *, Andreas Kacaras, Patrick Neuenfeldt, Volker Schulze (2) Karlsruhe Institute of Technology (KIT), wbk Institute of Production Science, Kaiserstr. 12, 76131 Karlsruhe, Germany

A R T I C L E I N F O

Keywords: Finishing Surface modiﬁcation Discrete element method

A B S T R A C T

The stream ﬁnishing process represents an efﬁcient mass ﬁnishing process capable in mechanical surface modiﬁcation. In order to generate a deeper understanding of the cause-effect relationships, normal forces, material removal and surface topography were analyzed and correlated for varied process parameters of disc-shaped AISI 4140 specimens. Local resolution of tangential velocities of the particles and normal forces on the workpiece’s surface were simulated using the discrete element method for deﬁned process parameter conﬁgurations and were correlated with experimental results. A deep process understanding is accomplished enabling the process design for efﬁcient surface smoothing and improved residual stress depth distribution. © 2019 Published by Elsevier Ltd on behalf of CIRP.

1. Introduction On the basis of fundamental parameters Hashimoto et al. established a comparison of a broad range of abrasive-ﬁne ﬁnishing processes and correlated them with surface integrity [1] revealing the potential of optimizing surface integrity due to mass ﬁnishing treatment [2]. In order to improve surface integrity of mechanical components a process design is mandatory which requires a deep understanding of material removal mechanisms depending on process parameters. Cutting and sliding effects occur during the mass ﬁnishing treatment [1] determining material removal Dm and leading both to plastic deformation effects and therefore to the induction of compressive residual stresses and work hardening into the sub-surface layer. Preston theoretically and experimentally investigated a plate glass polishing process [3] and proposed the hypothesis of a proportionality between the material removal Dm and the product of contact pressure p, relative velocity vrel and processing time t. According to [1] for pressure-copying processes Preston’s equation can be applied for the expression of the material removal rate. Due to the fact that mass ﬁnishing processes represent a group of pressure-copying processes the applicability of Preston’s equation is valid [1]. However, Brocker [4] could not conﬁrm the validity of Preston’s law for the unguided vibratory ﬁnishing process but a qualitative relationship between the power equivalent P = FN ∙ vrel, where FN stands for the normal force and vrel was assumed to be the tangential velocity vt, and the material removal was demonstrated. Despite the proportional relationship

* Corresponding author. E-mail address: [email protected] (F. Zanger). https://doi.org/10.1016/j.cirp.2019.04.086 0007-8506/© 2019 Published by Elsevier Ltd on behalf of CIRP.

is still unproven for mass ﬁnishing processes, P shows great potential for process design and its correlation with surface integrity. Furthermore, in order to describe material removal mechanisms the knowledge of occurring contact forces and velocities during mass ﬁnishing is mandatory. Besides [4], Yabuki et al. [5] and Hashimoto et al. [2] for the unguided vibratory ﬁnishing process as well as Ciampini et al. [6] for the guided vibratory ﬁnishing process contributed to the understanding of the occurring material removal mechanisms. The measurement of contact forces [2,4–6], velocities [4,6], contact modes [5] and impact frequencies [6] were conducted by them. A correlation between process parameters and contact conditions was established by [2,4,6]. Besides the surface topography further surface states were not considered. During mass ﬁnishing the media’s spatial ﬂow formation determined by process parameters and workpiece shape imply locally differing contact conditions which was shown by [6] for the guided vibratory ﬁnishing. However, a more complex spatial ﬂow formation due to impoundment effects is seen for the drag ﬁnishing process investigated by Uhlmann et al. [7] and the stream ﬁnishing process investigated by Schulze et al. [8] and Kacaras et al. [9] making the consideration of local contact conditions mandatory. The discrete element method (DEM) proved the capability in locally describing the contact behavior between media and workpiece but was only conducted with a signiﬁcantly reduced amount of particles, yet [7] and Kang et al. [10]. However, in order to describe the spatial ﬂow formation during stream ﬁnishing a more realistic amount of particles is mandatory. Therefore, approaches enabling an efﬁcient and realistic process description for mass ﬁnishing processes are necessary. Scientiﬁc gaps mentioned will be closed within the present paper for disc shaped AISI 4140 specimen by investigating cause-

F. Zanger et al. / CIRP Annals - Manufacturing Technology 68 (2019) 373–376

374

effect relationships between process parameters, contact conditions and surface integrity during stream ﬁnishing. The conducted experimental and simulative process analyses enable an advanced understanding for surface modiﬁcation and process design applicable to mass ﬁnishing processes in general. 2. Experimental setup and discrete element modeling For experiments a stream ﬁnishing machine SF1 68 (Otec Präzisionsﬁnish GmbH) was used. A high density sintered alumina ceramic KXMA 16 with an average grain size of 1.7 to 2.4 mm wetted with water and compound SC15 served as media. Fig. 1 schematically illustrates the stream ﬁnishing machine, the process parameters and the workpiece holder for the evaluation of Dm. Disc shaped, quenched and tempered AISI 4140 specimen (EN steel 1.7225) austenized at 850 C, quenched in oil and tempered at 450 C for 2 h with a diameter of 50 mm were ﬁnished. In order to evaluate local FN piezo resistive force sensors (FlexiForce A201, force range 0 to 111 N, Tekscan Inc.) were attached at three different positions. One in the center of the disc and the two remaining sensors horizontally shifted at 17 mm. The force signals were ampliﬁed and digitized at 32 Hz. A linear curve ﬁt was used for sensor calibration. Comparable sensor equipment has proven to be suitable to investigate contact forces during vibratory ﬁnishing by Ref. [5]. In order to evaluate the inﬂuence of process parameters on local FN the height above the bowl bottom z, the rotational speed n, the angle of immersion ’ and the workpiece orientation g were varied over a broad parameter range (Table 1). The radius of immersion r was kept constant at 270 mm in order to achieve the maximum possible relative ﬂow velocity between workpiece and media. Media distribution is inﬂuenced by the process parameters. Therefore, for each parameter conﬁguration the media distribution was measured using a laser distance sensor with a horizontal interval of 10 mm during ﬁnishing. Additionally, local Dm at the pos. 1 to 3 were evaluated using a speciﬁcally designed workpiece holder and attachable inserts with a diameter of 9.4 mm enabling a proportion of 94% planar material removal to 6% edge rounding, characterized by white light interferometry. Arithmetic average roughness Sa was analyzed with the same equipment as in Ref. [8] and a Gaussian ﬁlter of lL = 25 mm. Residual stress depth distributions were analyzed by X-ray stress analysis analogously to Ref. [8]. The model was created in the Rocky DEM (ESSS) software by abstracting the rotationally symmetrical processing bowl through a linear analogy channel with the same cross-section containing 1.25 E6 particles. The particle movement is induced by moving walls, whereby the radial speed change within the bowl is modeled by applying a corresponding speed proﬁle. The characteristic particle distribution over the cross-section of the bowl due to the centrifugal force is generated by the implementation of a

gravitational acceleration equivalent normal to the outer wall derived from the occurring circumferential velocity and radius of the bowl. Moreover, gravitational acceleration was implemented. Symmetry planes are located at the open channel ends, whereby outﬂowing media is returned to the calculation zone at the inlet of the channel. The media is modeled by spheres with a diameter of 2 mm corresponding to the mean particle size. The bulk density was determined to be 2310 kg m3. For contact modeling a hysteretic linear spring normal force model, a linear spring coulomb tangential force model and an elastic plastic rolling resistance model were used. The static and dynamic coefﬁcients of friction, the coefﬁcient of restitution as well as the Young’s modulus E basically correspond to dry alumina [11–13]. In order to reduce computing time by increasing the required time step the common simpliﬁcation of reducing the particle’s Young’s modulus [14,15] by a factor of 1 E3 was used. As a result signiﬁcantly reduced FN on the workpiece’s surface are calculated using the described model. However, Stewart et al. [15] showed for the DEM simulation of a granular ﬂow that this signiﬁcant downscaling provides comparable particle’s velocity vectors and ﬂow formation to experiments. This implies the validity of the used DEM model for qualitatively describing cause-effect relationships despite reduced FN level under the premise of a constant factor of reduction (addressed in Section 3.2). A correlation of simulatively determined local FN with experiments and simulated local vt values at the workpiece’s surface were evaluated for enhanced interpretation of experiments in Section 3.2. 3. Results and discussion 3.1. Normal force measurement and analysis Fig. 2 illustrates the measured FN and effective depths of immersion heff for the pos. 1 to 3 depending on the rotational speed n, the height above the bowl bottom z and for constant angles of immersion ’ and workpiece orientation g being both 0 (a). Furthermore, the inﬂuence of heff on FN is illustrated (b). Increasing FN and heff can be obtained for all positions with decreasing z. FN at the pos. 1 and 2 show to be slightly affected by n whereas forces at pos. 3 signiﬁcantly increase with growing n. Similar observations were made for ’ = 45 where comparable maximum forces occur at highest heff and n. However, forces for ’ = 45 at n={30,50} min1 turn out to be up to 30% higher compared to ’ = 0 implying a decreasing effect of n for growing ’. Considering the change of the vectorial force distribution due to p growing ’, FN,45 = ( 2⁄2) ∙ FN,0 is expected. Additionally, due to the reduced projected area of the workpiece normal to the ﬂow direction reduced impoundment effects and thus a further decrease of FN is expected. The discrepancy between measured and expected results can be explained by the fact that the

Fig. 1. Schematic view of the stream ﬁnishing machine with process parameters and the workpiece holder for the evaluation of local Dm.

Table 1 Investigated parameter range. Process parameter

z/mm

n/min1

’/

g /

Tested values

150 to 75

30 to 90

0 to 45

50 to +50

Fig. 2. Measured local FN and heff depending on deﬁned process parameters (a) and local FN in dependency on heff with linear ﬁts (b).

F. Zanger et al. / CIRP Annals - Manufacturing Technology 68 (2019) 373–376

workpiece orientation leads to a media ﬂow deﬂection towards the bowl bottom and thus to higher static pressure ﬁelds determined by centrifugal and gravitational forces. As a result impoundment effects increase leading to an increase of FN. At pos. 3 the highest dependency of FN and heff on n is obtained leading to an increasing force distribution on the workpiece’s surface with growing n. The inhomogeneous FN and heff suggest a proportionality between both process values. Fig. 2b shows a clearer representation of the dependency between local FN and heff for ’ = 0 and all tested n and z. The local dependency of both values for each n can be described sufﬁciently good using a linear ﬁt (R2 ranging from 0.94 to 0.99) showing similar slopes. A signiﬁcantly higher slope of a ﬁt for the pos. 1 and 3 (exemplarily for n = 90 min1 and z = 75 mm) implies that the inhomogeneous FN cannot be traced back to the inhomogeneous heff solely. Consideration of local forces in combination with local velocities is essential at this point for the explanation of this effect which is addressed in Section 3.2. The inﬂuence of g on local FN for both tested ’ are shown in Fig. 3 for the parameter conﬁguration showing highest FN in Fig. 2a. Furthermore, simulatively determined normalized vr which describe the local velocity vector components in r-direction of the bowl for ’ = 0 and selected values of g are depicted (simulation model is discussed in Section 3.2). FN show comparable values depending on g for both ’ and are thus consistent to the previously mentioned observation. Increasing g analogously to increasing ’ leads to a forced ﬂow deﬂection due to workpiece orientation towards higher static pressure ﬁelds resulting in increased FN. vr values indicate a transition of the ﬂow direction on the workpiece’s surface at g = 20 . For positive vr the media ﬂow is deﬂected towards the wall of the bowl and vice versa. With increasing g a shift of the ﬂow’s stagnation point (vr 0) from pos. 3 to 1 occurs leading to the peak of FN at pos. 3. Due to the shift of the stagnation point and the correlation with FN an inversely proportional relation between FN and vt in dependence on g is expected. This hypothesis will be addressed in Section 3.2.

375

While the average ﬂow direction shows comparable values in xdirection varying ﬂow directions in y-direction (local axis system of the workpiece) can be obtained in Fig. 4a. Flow directions correlate well with experimentally determined groove directions (Fig. 6b) and will be discussed in Section 3.3. For all parameter conﬁgurations simulated FN were calculated to be 80 to 92% lower than the experimentally determined FN. The small deviations of the factor of reduction imply the suitability of the model for the qualitative description of cause-effect relationships. Simulated normalized FN and vt and corresponding normalized P during stream ﬁnishing for deﬁned process parameter conﬁgurations are illustrated in Fig. 5. Cause-effect relationships between experimentally (Section 3.1) and simulatively determined FN for identical process parameter conﬁgurations show a strong consistency. While a slight tendency to an increase of vt can be obtained for growing n and z, results show vt to be signiﬁcantly affected by ’ and g . Results indicate that the process parameters ’ and g allow the effective manipulation of occurring FN and vt and thus the resulting mechanical loading during stream ﬁnishing. Locally increasing vt and decreasing FN imply a local decrease of impoundment effects. Therefore, the inhomogeneous force distribution shown in Fig. 2b can be traced back to locally differing impoundment effects. Analysis of the power equivalent P = FN ∙ vt is addressed in Section 3.3. An increase of g leads to growing FN at the pos. 1 and 2 while FN at pos. 3 shows a peak value and thus is consistent to the results in Fig. 3. The values of vt in dependence on g show an inversely proportional relation to FN which veriﬁes the hypothesis stated in Section 3.1. 3.3. Material removal and surface integrity Experimentally determined Dm at the pos. 1 to 3 and roughness change after 20 min of stream ﬁnishing are depicted in Fig. 6a.

3.2. Discrete element simulation and correlation with experiments According to Ref. [3] the consideration of FN and vt is mandatory in order to describe process efﬁciency in terms of material removal and effects described in Section 3.1. As occurring local vt are practically hard to measure because of the media’s opaqueness and the strong abrasive effects DEM simulations were conducted. Fig. 4 shows simulated velocity vectors (a) and a comparison of simulated and experimentally determined local FN for a single condition (b) during stream ﬁnishing using the parameter conﬁguration showing highest FN in Fig. 2a exemplarily.

Fig. 5. Simulated normalized FN and vt and corresponding P during stream ﬁnishing for deﬁned process parameter conﬁgurations.

Fig. 3. Local FN depending on ’ and g with normalized vr for ’ = 0 .

Fig. 4. Simulated velocity vectors (a) and a comparison of simulated and experimentally determined local FN (b) during stream ﬁnishing with g = ’ = 0 , z = 75 mm and n = 90 min1.

Fig. 6. Local Dm and roughness change for deﬁned parameter conﬁgurations (a) and surface texture directions for g = ’ = 0 , z = 75 mm and n = 90 min1 (b) before and after 20 min of ﬁnishing.

376

F. Zanger et al. / CIRP Annals - Manufacturing Technology 68 (2019) 373–376

Fig. 6b illustrates the Fast Fourier Transform of 3-dimensional surface topography measurements at different positions before and after 20 min of stream ﬁnishing using a polar diagram. Additionally, the groove direction range derived from heff for the pos. 1 to 3 are implemented. A temporal change of material removal rate occurs during the transient roughness period [8]. Therefore, in order to state a valid comparison of resulting Dm in dependence on process parameter conﬁgurations, a processing time leading to a stationary roughness state is mandatory. After 20 min of stream ﬁnishing roughness reduction occurs with a resulting Sa ranging between 0.05 to 0.07 mm. Regardless signiﬁcantly differing Dm for varying process parameters the resulting Sa values attain a stationary roughness state for all tested parameter conﬁgurations. Change in ’ or g leads to a reduction in projected area of the workpiece normal to the ﬂow direction of the media. Theoretically, a quadratic relation between p and the r-direction due to the centrifugal inﬂuence and a linear relation between p and the direction towards the bowl bottom (decreasing z) due to the gravitational inﬂuence is given. Therefore, forcing the media ﬂow in an increasing radial direction, a larger pressure gradient and thus higher impoundment effects in comparison to a forced media ﬂow in the direction of the bowl bottom occur. Despite the deﬂection of the media ﬂow in depth direction impoundment effects are lower compared to a frontal inﬂow (’ = g = 0 ). This is in accordance with the increasing vt with increasing ’ and decreasing g (Fig. 5). Before stream ﬁnishing, the workpiece was attached to the workpiece holder with a vertically oriented groove direction. Due to the point symmetry of the texture directions to the origin, the polar diagram in Fig. 6b is displayed from 0 to 180 . The surface shows different local preferred texture directions depending on the pos. a, 2 and b which correlate with simulated results in Fig. 4. The groove direction range of heff which can theoretically be seen as the direction of the highest pressure gradient is largely in accordance with the experimentally determined texture directions. Highest Dm values can be achieved by proﬁciently setting of ’ or g. The initial assumption of the applicability of Preston’s law is valid due to the presence of dominating planar material removal described in Section 2 with a uniform pressure over the insert’s contact area. However, the P/Dm ratios show a percentage standard deviation of nearly 68% from the mean value demonstrating the hypothesis proposed by Ref. [3] not to be valid for the stream ﬁnishing process and conﬁrm the results of Ref. [4]. In order to determine the qualitative relation, Pearson correlation coefﬁcients between the calculated P and measured Dm were calculated. Correlation coefﬁcients for pos. 1 to 3 ranging between 0.87 and 1 show an evidence for linearity. For varied n at ’ = g = 0 both values at pos. 3 show no strong correlation which can be traced back to the relatively low Dm in combination with the standard deviations. However, P proves to be a valid qualitative measure for Dm and thus to asses process efﬁciency. Residual stress (s RS) depth distributions measured at pos. 2 of workpieces before and after stream ﬁnishing using parameter conﬁgurations showing highest Dm are displayed in Fig. 7. Assuming that P is a measure for the processing intensity and mechanical effects dominate (temperature effects are negligible), higher induced compressive s RS are expected with increasing P in analogy to an increasing processing intensity [9]. Considering that

Fig. 7. s RS states at pos. 2 before and after ﬁnishing using varied parameter conﬁgurations with n = 90 min1 and t = 20 min and P values.

depth distributions are only reasonable down to a depth of 5 mm because electrochemical polishing has an accuracy of 2 mm which accumulates per depth step, the above mentioned assumption can clearly be conﬁrmed. 4. Conclusion A comprehensive correlation between process parameters, local contact conditions and surface integrity was established for disc shaped AISI 4140 specimen during stream ﬁnishing using the synergy of experimental and simulative analyses. Results enable an advanced process understanding regarding cause-effect relationships and contribute to an advanced process design for surface modiﬁcation by means of mass ﬁnishing treatment in general. Following key ﬁndings can be stated: Preston’s law did not show to be applicable but the power equivalent P = FN ∙ vt proved to be a valid qualitative measure for Dm and induced compressive residual stresses s RS and thus to assess process efﬁciency. For a process design the local consideration is mandatory due to an inhomogeneous FN and vt distribution related to impoundment effects. These can be effectively inﬂuenced by the angle of immersion ’ and the workpiece orientation g inﬂuencing FN and vt and thus the resulting mechanical loading and process efﬁciency. Local FN showed to be a linear function of the effective depth of immersion heff arising from the increasing static pressure. An increase of n per se leads to an increase of FN and vt due to an increase of the kinetic energy of particles but can locally be compensated by impoundment effects.

Acknowledgements The authors thank the German Research Foundation (DFG) for the funding of the research project (SCHU 1010/62-1), Otec Präzisionsﬁnish GmbH for the ﬁnancial support and Dr. Gibmeier from IAM-WK of KIT for measuring the residual stresses.

References [1] Hashimoto F, Yamaguchi H, Krajnik P, Wegener K, Chaudhari R, Hoffmeister HW, Kuster F (2016) Abrasive Fine-Finishing Technology. CIRP Annals – Manufacturing Technology 65:597–620. [2] Hashimoto F, Johnson SP, Chaudhari RG (2016) Modeling of Material Removal Mechanism in Vibratory Finishing. CIRP Annals – Manufacturing Technology 65:325–328. [3] Preston FW (1927) The Theory and Design of Plate Glass Polishing Machines. Journal of the Society of Glass Technology 11:214–256. [4] Brocker R (2015) Relativgeschwindigkeiten und Kontaktkräfte beim ungeführten Vibrationsgleitschleifen, Dissertation RWTH Aachen University. [5] Yabuki A, Baghbanan MR, Spelt JK (2002) Contact Forces and Mechanisms in a Vibratory Finisher. Wear 252:635–643. [6] Ciampini D, Papini M, Spelt JK (2007) Impact Velocity Measurement of Media in a Vibratory Finisher. Journal of Materials Processing Technology 183:347–357. [7] Uhlmann E, Eulitz A, Dethlefs A (2015) Discrete Element Modelling of Drag Finishing. Procedia CIRP 31:369–374. [8] Schulze V, Gibmeier J, Kacaras A (2017) Qualiﬁcation of the Stream Finishing Process for Surface Modiﬁcation. CIRP Annals – Manufacturing Technology 66:523–526. [9] Kacaras A, Gibmeier J, Zanger F, Schulze V (2018) Inﬂuence of Rotational Speed on Surface States After Stream Finishing. Procedia CIRP 71. 332–226. [10] Kang YS, Hashimoto F, Johnson SP, Rhodes JP (2017) Discrete Element Modeling of 3D Media Motion in Vibrator Finishing Process. CIRP Annals – Manufacturing Technology 66:313–316. [11] Poser K, Zum Gahr KH, Schneider J (2005) Development of Al2O3 Based Ceramics for Dry Friction Systems. Wear 259:529–538. [12] DellaCorte C, Pepper SV, Honecy FS (1991) Tribological Properties of Ag/Ti Films on Al2O3 Ceramic Substrates. NASA Technical Memorandum 103784. [13] Blau PJ (2008) Friction Science and Technology – From Concepts to Applications, CRC Press Taylor & Francis Group. ISBN:978-14200-5404-0. [14] Washino K, Chan EL, Tanaka T (2018) DEM with Attraction Forces Using Reduced Particle Stiffness. Powder Technology 325:202–208. [15] Stewart RL, Bridgwater J, Zhou YC, Yu AB (2001) Simulated and Measured Flow of Granules in a Bladed Mixer – A Detailed Comparison. Chemical Engineering Science 56:5457–5471.

Copyright © 2023 C.COEK.INFO. All rights reserved.